Homogeneous superconducting phase in TiN film: A complex impedance study
P. Diener, H. Schellevis, and J. J. A. Baselmans
Citation: Appl. Phys. Lett.101, 252601 (2012);
View online: https://doi.org/10.1063/1.4771995
View Table of Contents: http://aip.scitation.org/toc/apl/101/25
Published by the American Institute of Physics
Articles you may be interested in
Coherent growth of superconducting TiN thin films by plasma enhanced molecular beam epitaxy
Journal of Applied Physics 112, 083920 (2012); 10.1063/1.4759019
Titanium nitride films for ultrasensitive microresonator detectors
Applied Physics Letters 97, 102509 (2010); 10.1063/1.3480420
Measurements of the Kinetic Inductance of Superconducting Linear Structures
Journal of Applied Physics 40, 2028 (2003); 10.1063/1.1657905
Photon-noise limited sensitivity in titanium nitride kinetic inductance detectors
Applied Physics Letters 106, 073505 (2015); 10.1063/1.4913418
Frequency-tunable superconducting resonators via nonlinear kinetic inductance
Applied Physics Letters 107, 062601 (2015); 10.1063/1.4927444
Proximity-coupled Ti/TiN multilayers for use in kinetic inductance detectors
Homogeneous superconducting phase in TiN film: A complex impedance
P. Diener,1,a)H. Schellevis,2and J. J. A. Baselmans1 1
SRON Netherlands Institute for Space Research, 3584 CA Utrecht, The Netherlands
Delft Institute of Microsystems and Nanoelectronics, Delft University of Technology, 2628 CD Delft, Netherlands
(Received 26 June 2012; accepted 28 November 2012; published online 17 December 2012)
The low frequency complex impedance of a high resistivity 92lXcm and 100 nm thick TiN superconducting film has been measured via the transmission of several high sensitivity GHz microresonators, down toTC=50. The temperature dependence of the kinetic inductance follows
closely BCS local electrodynamics, with one well defined superconducting gap. This evidences the recovery of a homogeneous superconducting phase in TiN far from the disorder and composition driven transitions. Additionally, we observe a linearity between resonator quality factor and frequency temperature changes, which can be described by a two fluid model.VC 2012 American
Institute of Physics. [http://dx.doi.org/10.1063/1.4771995]
Thin films of titanium nitride (TiN) have recently been proposed1 for radiation detection using kinetic inductance detectors.2TiN and other strongly disordered superconduct-ing materials have a high surface impedance for radiation with a photon energyh >2D, which allows highly efficient radiation absorption. Additionally, disordered superconduc-tors have a long magnetic penetration depth. This results in a relatively large value of the kinetic inductance, which increases the responsivity of the devices.
Recent work has revealed strong deviations from stand-ard BCS theory for superconductors with a normal state re-sistivity in the range of 100lXcm and higher,3 clearly in violation of the Anderson theorem, which states that disorder does not affect the properties of the superconducting state.4 These deviations increase with higher disorder, leading to systems in which a superconductor insulator transition (SIT) is observed, typically when the Ioffe-Regel parameter kF‘1. SITs have been observed in thin films of several
materials by changing the disorder via a film treatment, or by varying the thickness, the film stoichiometry or the applied magnetic field.5–8 In TiN, a SIT has been evidenced few years ago in5 nm thick films by magnetic field and thick-ness changes.9,10Several studies also report the presence of an inhomogeneous superconducting phase close to the SIT.11–15
One expects to recover a classical BCS superconducting phase when going to lower disorder/thicker films. In contrast, the only one spectroscopic study on a low disordered TiN film reports on the presence of a non uniform state compris-ing of superconductcompris-ing and normal areas.16These results are discussed in the context of mesoscopic fluctuations close to a superconducting to normal transition. Indeed, TiN also exhibits a transition with composition: as reported recently, superconductivity disappears in the N sub stoichiometric range.1The presence of an inhomogeneous order parameter in a low disordered TiN film points out the necessity to dis-entangle the thickness and composition transitions.
In this paper, we report on the complex impedance study of several microresonators made of a 100 nm thick, relatively weakly disordered TiN film, having kF‘¼12:7 and a
resis-tivity of 92lXcm. The film has been characterized exten-sively, and the resonators have internal quality factors up to 107. This allows an accurate determination of the supercon-ducting gap from the temperature resonance frequency shift, which is directly proportional to the kinetic inductance or superfluid density changes.
The film has been prepared by a DC magnetron sputter-ing system. It is sputtered on a nitrogen/argon plasma at 350C on a high resistive HF cleaned silicon substrate (see Ref. 17 for more details on the recipe). The thickness determined with a scanning electron microscope is d¼10065 nm. The homogeneity has been checked by X-ray photoelectron spectroscopy (XPS) depth profiling: as shown in Fig.1, there is no contamination except some oxy-gen at the surface on few nm, and the Ti/N ratio is thickness independent. The stoichiometry determined is 1:1.3 with an uncertainty of 20% related to the XPS calibration. There is a 1 GPa stress in the film, to obtain a dense and homogeneous
FIG. 1. Concentration-depth profiles measured by XPS depth profiling. The sputter rate calibrated in SiO2at the used setting of the ion gun was 4.4 nm/
min. A small oxygen contamination is observed at the surface (left) on few nm, and the Ti and N concentrations remain constant in the film up to the Si substrate (right). The measured stoichiometry is 1:1.3 with, however, an im-portant error due to the 20% uncertainty on the absolute concentration val-ues with this technique.
granular morphology.17 This affects the unit cell size of 4:35A determined by X-ray diffraction (XRD), to be com-˚ pared to the bulk value 4:24A. XRD spectra also show a˚ favored (200) crystalline orientation. A typical grain size of 10 nm has been determined by transmission electron micros-copy in others TiN films from the same source.17
The film characterizations at low temperature include standard R(T) and Hall measurements. The resistivity at 10 K, q¼92lXcm is almost constant up to 300 K and the carrier density isn0¼3:771022cm3.kF‘can be estimated in the
free electron model from q and n0 by18 kF‘¼3p2h
Þ giving 12.7 for this film. In addition, Fig. 2
shows the sharp superconducting transition observed at TC¼4:3860:01 K.
Coplanar waveguide resonators (CPW) have been pat-terned using standard contact lithography and dry etching with an SF6=Ar gas mixture. One resonator is shown Fig.2. The resonators are formed by a central meandered line of few mm length, 3lm wide, and slits of 2lm wide between the central line and the groundplane. They are capacitively coupled to the feedline by placing one resonator end along-side it. The feedline is connected to coaxial cables at both chip sides and itsS21transmission is measured using a stand-ard vector network analyzer. A detailed description of the setup can be found in Ref.19.
Each resonator gives rise to a dip in S21 at a frequency f01¼2pxl
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðLkþLgÞC p
, withlthe resonator length,Lk and
Lgthe kinetic and geometric inductance per unit length, and
Cthe capacitance per unit length.xis a factor depending on the resonator type. Here, half of the resonators are halfwaves (open ended on both sides) corresponding tox¼2, the others are quarterwaves (short ended on one side) thusx¼4. The inductance per unit length is proportional to the surface in-ductance:Ls¼Lk=gwith g a factor depending on the
resona-tor geometry.3 When the temperature is increased, Cooper pairs are broken by thermal excitations above the gap,
result-ing in a change of the kinetic inductance. This translate into a resonance frequency shift (see Fig.2) and
withaLk=ðLkþLgÞthe kinetic inductance ratio. For high
LkLg films like the TiN film studied here, a is large
enough to be determined precisely from the ratio of the ex-perimental resonance frequency at the lowest temperaturef0 and the geometrical frequency fg calculated from the CPW
To choose the correct model forLsðTÞ, we first estimate
several characteristic lengths. The London magnetic penetra-tion depth kL47 nm is determined from the measured n0
and using a quasiparticle massmequal to 3 times the electron mass.21The BCS coherence lengthn0¼hvF
pD120 nm is esti-mateda prioriusing a gapD¼1:76kBTCand a Fermi
veloc-ity vF¼ hp3ﬃﬃﬃﬃﬃﬃﬃﬃﬃ3p2n0
m . The mean free path ‘¼svF¼ m
vF1 nm is calculated from the measured.0andn0. We are now in position to estimate the effective coherence length nef f ¼ ðn10 þ‘
1Þ11:0 nm and the magnetic penetration
depthkef f ¼kLð1þn0‘Þ
517 nm. The film studied here is in the local (nef f kef f), dirty (‘ n0;kL), three
dimen-sional (nef f d) and thin film limit (d kef f). In thin films,
the current is distributed uniformly and the relation between the square inductance andkef f simply reduces to
Ls¼l0 k2ef f
d : (2)
In the local dirty limit and at T<Tc=3, the temperature
dependence ofkef f is given by22
¼tanh D0 2kBT
withD0 the superconducting gap at zero temperature. This is valid in the low frequency limithf 2D0. It is verified here, since the frequency range used is 3–5.3 GHz corresponding to 12–22leV, which is less than 2% of the gap energy. Com-bining Eqs.(1)–(3), one obtains
f0 ¼2 tanh
where f, Ls, and kef f have been replaced by their value
at the lowest experimental temperature f0;Ls0, and keff0 which is correct fordLðsÞ Ls0 and dkef fðTÞ keff0. This
is valid for all temperatures below T0:9Tc, temperature
above which the magnetic penetration depth diverges. As shown in Eq. (4), the temperature dependence of the reso-nance frequency shift is a direct probe of the superconduct-ing gap.
The S21 transmission of 8 resonators of the same chip has been measured between 90 mK and 1 K. At low tempera-ture, the internal quality factors are between 106 and 107. These high values support the conclusions of Ref. 23on the relation between high quality factors and a (200) crystalline orientation in TiN films. Theðf0=fgÞratio calculated from the
FIG. 2. TypicalS21 transmission of one resonator for several temperatures
between 90 mK and 1 K. When increasing T, the frequency and the quality factor decrease due to quasiparticle excitations above the gap. Upper inset: resistive superconducting transition. Lower inset: photo of one resonator from another chip having the same design. The meandered resonator line (light grey) is separated to the groundplane all around (light grey) by slits (dark grey) and is capacitively coupled to the feedline (lower straight line).
measured f0 is the same for all resonators, giving a¼1 ðf0=fgÞ
¼0:69. dLs=Ls0ðTÞ is shown in Fig. 3 for all resonators. They exhibit the same temperature depend-ence and an excellent fit is obtained with Eq. (4), giving
D¼0:57 meV. There is, however, a slightly weaker curva-ture of the measureddLs=Ls0ðTÞbelow 0.6 K, which is mag-nified in log scale in the inset. The curves are between the values expected for D¼0:48 meV and D¼0:57 meV, which may be attributed to a small gap decrease close to the film surfaces due to oxidization or stoichiometry changes, see Fig.1. The inflexion point aroundT0:45 K, followed below by a cut-off of the inductance shift which is not identi-cal for all resonators/frequencies, is due to the capacitive dielectric variations24 which becomes non negligible com-pared to the inductive changes in this temperature range. ComparingDand the critical temperatureTC¼4:38 K, one
obtains a ratio D=kBTC¼1:50, lower than the BCS weak
coupling ratio 1.76. This has nothing to do with the SIT: in contrast, as observed by Sacepe et al. in TiN ultra thin films,12 one expects disorder to possibly increase D=kBTC
close to the transition. The 1.50 ratio may be related to an effect of the grain size: as reported by Boseet al.25in nio-bium thick films, the critical temperature decreases when decreasing the grain size and the D=kBTC ratio is slightly
reduced, going to 1.61 for 18 nm grains. A superconductivity weakening can also occur due to interface tunnel exchange at internal and external surfaces26 as observed in niobium thin films.27 This may also explain why all TC reported for
TiN films are below 4.8 K, whereasTC¼6:0 K in a TiN
To go further, we have also compared the temperature dependence of the frequency and the quality factorQ. Fig.4
shows the temperature dependence of the normalized quality factorsdð1=QÞðTÞ ¼ ð1=QÞðTÞ ð1=QÞðT¼0Þfor all reso-nators as a function of the frequency shift—df(T). The 8 res-onators give similar results, and exhibit a linear behaviour. In the following, we show how this proportionality between quality factor and frequency shift can be reproduced analyti-cally in the context of the two fluid model. In general, the ra-dio frequency absorption cannot be described by local
electrodynamics even at low temperature and low frequency, due to the non trivial form of the momentum transition ma-trix M.29This holds here, however, since we are only inter-ested in the temperature dependencedð1=QÞðTÞand because M is temperature independent at T<Tc=3, where the gap
and BCS coherence length remain unchanged.
Q is related to the surface impedance ZS¼RSþixLS
byQ¼xLtotal=Rtotal¼xLS=aRS, withRS the surface
resist-ance. In the thin film limit,ZS is simply related to the
com-plex conductivity r¼r1þir2 by Zs1¼rd. At low
temperature, r1 r2 and we get RS¼rr12 2d
and LS ¼xr21d.
The complex conductivity in the two fluid model is given by22
m 1 1ixsþi
withnnthe quasiparticle density andsthe momentum
relax-ation time. In the limit xs 1, one gets for the quality factor
The first part of Eq.(6)is identical to the equation used by Gao et al.30 in the context of the Mattis Bardeen theory. Using the propertiesnn¼dnn;dnn=dns¼ 2, it becomes
QðTÞ ¼ 2axs dnSðTÞ
The quality factor temperature dependence is directly related to the superfluid density changes, as for the kinetic induct-ance:LSðTÞ ¼2nSðmTÞe2dand
f : (8)
By combining Eqs. (7) and (8), we obtain the relation between Q anddf
Q¼ 8ps df: (9)
As shown in Eq.(9), the inverse quality factor is proportional to the frequency shift and momentum relaxation time. This FIG. 3. Temperature dependence of the normalized surface inductance for
the 8 resonators, havingf0¼3:28 GHzð䊏Þ, 3.36 GHz (䊉), 3.41 GHz (䉱),
3.46 GHz (䉲), 3.52 GHz (䉬), 4.79 GHz (䉳), 5.01 GHz (䉴), 5.23 GHz (䊉). The black line is the best fit with Eq. (4) giving the gap value
D¼0:57 meV. Inset: same curves in semi-log and inverse temperature scales to magnify the results at the lowest temperatures. The dotted line is Eq.(4)withD¼0:48 meV.
means that losses, which are expected to be zero at zero tem-perature, increase proportionally to the quasiparticle density changes df /dnn, via the two fluid property dnn/dns. In
practice, there are always residual losses 1/Q(T¼0) due to non equilibrium excess quasiparticles,31,32 which are sub-tracted in Fig.4. Fitting the results with Eq.(9)gives the mo-mentum relaxation time atT Tc;s¼1:7 1012s. This is
three orders of magnitude longer than in the metallic state sm¼m=n0e2q¼3:01015s estimated from the
resistiv-ity and the carrier densresistiv-ity measured at 10 K. In the supercon-ducting state, indeed, the momentum relaxation time strongly increases, typically up to 1012s in usual BCS superconductors22 due to the quasiparticles vanishing by Cooper pair condensation.
The temperature dependence of the resonators’ frequen-cies and quality factors clearly evidences the presence of one well defined superconducting gap in the density of states. Moreover, the excellent reproducibility between the resona-tors evidences the good superconducting phase homogeneity in the film. This differs from previous STM/S results on a similar 100 nm thick high TC¼4:68 K TiN film, which
report on the presence of an inhomogeneous superconducting phase having local normal areas. As discussed in Ref.16, the detected inhomogeneous gap may be due to mesoscopic fluctuations at the proximity of a superconductor to metal transition. Indeed, the presence of a composition driven tran-sition in TiNxhas been reported recently,1with a
disappear-ance of the superconducting phase in the low x range, recovered atx¼0 (titanium). However, the film used in Ref.
16 has the characteristic high critical temperature of over-stoichiometric TiN, similar to the one of the film measured here, and our results do not exhibit any signature of the proximity with the composition transition. Additionally, the granular morphology of the two films is different. Indeed, the film recipe used here has been especially developed to obtain densely packed grains in the film, corresponding to zone T in the Thornton classification. As discussed in Ref.
17, a typical low stress TiN film is of zone 1, containing many voids between grains. This may lead to important Josephson barriers between superconducting grains, which are expected to play a major role in the homogeneity of the superconducting phase of such systems even at relatively low disorder.33
In conclusion, the low frequency complex surface im-pedance has been studied on microresonators made from a thick overstoichiometric TiN film. The resonators’ high qual-ity factors allow a high sensitivqual-ity determination of the in-ductive and resistive changes with temperature. In contrast to the previous spectroscopic study in a similar film, all our results are in agreement with a homogeneous superconduct-ing phase havsuperconduct-ing a gapD¼0:57 meV¼1:50kBTC.
We thank T. M. Klapwijk, A. Endo, E. F. C. Driessen, P. C. J. J. Coumou, R. R. Tromp, and S. J. C. Yates for sup-port and fruitful discussions.
1H. G. Leduc, B. Bumble, P. K. Day, B. H. Eom, J. Gao, S. Golwala, B. A.
Mazin, S. McHugh, A. Merrill, D. C. Mooreet al.,Appl. Phys. Lett.97, 102509 (2010).
P. K. Day, H. G. LeDuc, B. A. Mazin, A. Vayonakis, and J. Zmuidzinas,
Nature425, 817 (2003).
3E. F. C. Driessen, P. C. J. J. Coumou, R. R. Tromp, P. J. de Visser, and T.
M. Klapwijk,Phys. Rev. Lett.109, 107003 (2012).
P. W. Anderson,J. Phys. Chem. Solids11, 26 (1959).
5D. Shahar and Z. Ovadyahu,Phys. Rev. B46, 10917 (1992).
6C. A. Marrache–Kikuchi, H. Aubin, A. Pourret, K. Behnia, J. Lesueur, L.
Berge, and L. Dumoulin,Phys. Rev. B78, 144520 (2008).
S. Okuma, T. Terashima, and N. Kokubo,Solid State Commun.106, 529– 533 (1998).
8E. Bielejec and W. Wu,Phys. Rev. Lett.88, 206802 (2002). 9
T. I. Baturina, D. R. Islamov, J. Bentner, C. Strunk, M. R. Baklanov, and A. Satta,JETP Lett.79, 337–341 (2004).
10N. Hadacek, M. Sanquer, and J.-C. Villegier,Phys. Rev. B69, 024505 (2004). 11T. I. Baturina, C. Strunk, M. R. Baklanov, and A. Satta,Phys. Rev. Lett.
98, 127003 (2007).
B. Sacepe, C. Chapelier, T. I. Baturina, V. M. Vinokur, M. R. Baklanov, and M. Sanquer,Phys. Rev. Lett.101, 157006 (2008).
13T. I. Baturina, J. Bentner, C. Strunk, M. Baklanov, and A. Satta,Phys. B: Condens. Matter359–361, 500–502 (2005).
T. I. Baturina1, A. Yu. Mironov, V. M. Vinokur, M. R. Baklanov, and C. Strunk,Phys. Rev. Lett.99, 257003 (2007).
15V. M. Vinokur, T. I. Baturina, M. V. Fistul, A. Y. Mironov, M. R.
Bakla-nov, and C. Strunk,Nature452, 613 (2008).
W. Escoffier, C. Chapelier, N. Hadacek, and J.-C. Villegier,Phys. Rev. Lett.93, 217005 (2004).
17J. F. Creemer, D. Briand, H. W. Zandbergen, W. van der Vlist, C. R. de Boer,
N. F. de Rooij, and P. M. Sarro,Sens. Actuators, A148, 416–421 (2008).
N. D. Ashcroft and N. D. Mermin,Solid State Physics(Brooks & Cole, 1976).
19J. J. A. Baselmans, S. Yates, P. Diener, and P. de Visser,J. Low Temp. Phys.167, 360–366 (2012).
J. Gao, J. Zmuidzinas, B. A. Mazin, P. K. Day, and H. G. Leduc,Nucl. Ins-trum. Methods559, 585–587 (2006).
21C. Walker, J. Matthew, C. Anderson, and N. Brown,Surf. Sci.412, 405–
M. Tinkham,Introduction to Superconductivity(McGraw-Hill, New York, 1996).
23M. R. Vissers, J. Gao, D. S. Wisbey, D. A. Hite, C. C. Tsuei, A. D.
Cor-coles, M. Steffen, and D. P. Pappas,Appl. Phys. Lett.97, 232509 (2010).
R. Barends, H. L. Hortensius, T. Zijlstra, J. J. A. Baselmans, S. J. C. Yates, J. R. Gao, and T. M. Klapwijk,Appl. Phys. Lett.92, 223502 (2008).
25S. Bose, P. Raychaudhuri, R. Banerjee, P. Vasa, and P. Ayyub,Phys. Rev. Lett.95, 147003 (2005).
J. Halbritter,Phys. Rev. B46, 14861 (1992).
27J. Halbritter,Solid State Commun.34, 675–678 (1980).
28W. Splengler, R. Kaiser, A. N. Christensen, and G. Muller-Vogt,Phys. Rev. B17, 1095–1101 (1978).
J. Halbritter,Z. Phys.266, 209–217 (1974).
30J. Gao, J. Zmuidzinas, A. Vayonakis, P. Day, B. Mazin, and H. Leduc, J. Low Temp. Phys.151, 557–563 (2008).
D. E. Oates, A. C. Anderson, C. C. Chin, J. S. Derov, G. Dresselhaus, and M. S. Dresselhaus,Phys. Rev. B43, 437655 (1991).
32P. J. de Visser, J. J. A. Baselmans, P. Diener, S. J. C. Yates, A. Endo, and
T. M. Klapwijk,Phys. Rev. Lett.106, 167004 (2011).
B. Spivak, P. Oreto, and S. A. Kivelson,Phys. Rev. B77, 214523 (2008).